New Colloidal Lithographic Nanopatterns Fabricated by Combining Pre-Heating and Reactive Ion Etching
- First Online:
- Cite this article as:
- Cong, C., Junus, W., Shen, Z. et al. Nanoscale Res Lett (2009) 4: 1324. doi:10.1007/s11671-009-9400-0
We report a low-cost and simple method for fabrication of nonspherical colloidal lithographic nanopatterns with a long-range order by preheating and oxygen reactive ion etching of monolayer and double-layer polystyrene spheres. This strategy allows excellent control of size and morphology of the colloidal particles and expands the applications of the colloidal patterns as templates for preparing ordered functional nanostructure arrays. For the first time, various unique nanostructures with long-range order, including network structures with tunable neck length and width, hexagonal-shaped, and rectangular-shaped arrays as well as size tunable nanohole arrays, were fabricated by this route. Promising potentials of such unique periodic nanostructures in various fields, such as photonic crystals, catalysts, templates for deposition, and masks for etching, are naturally expected.
KeywordsNanosphere lithography Nanopatterns Reactive ion etching Preheating Nonspherical Nonclose-packed
Assembling colloidal micro/nano particles into 2-dimensional (2D) or 3-dimensional (3D) ordered arrangements has been of considerable importance in potential applications to biochips and biosensors [1–3], chemical sensors, optical and electronic devices , photonic crystals and suface wettability [5, 6], and as templates for designed nanostructures for magnetic data storage memory bits, and surface-enhanced Raman scattering substrates, etc. [7, 8]. A variety of nanofabrication technologies have been developed to prepare large-area 2D or 3D colloidal patterned surfaces, such as self-assembly, spincoating, electric-field-induced electrokinetic flowing, and Langmuir-Blodgett deposition [9–14]. In particular, self-assembly technique, which forming ordered periodic arrays of packed spherical configuration with uniformly sized microspheres, has been applied widely because of its unique features: it is inexpensive, inherently parallel, and enables high-throughput nanofabrication. The template formed by the self-assembly of monodisperse nanospheres on flat surfaces can be used as an etching/deposition mask to fabricate a periodic array of nanosized particles with a technique known as nanosphere lithography (NSL). However, self-assembly alone is greatly restricted to the formation of close-packed spherical pattern. Therefore, one disadvantage of NSL is its limited pattern design. Only triangular-shaped metal nanoparticles can be directly obtained from deposition through monolayer and double layer of close-packed nanospheres.
To extend the limited patterns of NSL, one method is shadow NSL, which is a combination of monolayer-preparation of PS spheres with tilted shadow evaporation [15, 16], the other one is to change the colloidal patterns. In recent years, reactive ion (plasma) etching (RIE) has been widely used to extend the close-packed spherical colloidal patterns based on self-assembly into nonclose-packed nonspherical patterns. It becomes more challenging to fabricate nonspherical particles with controllable shapes, nonclose-packed patterns, and good periodicity in a large scale. Choi et al.  employed RIE technique with pure O2 gas or mixture of CF4 and O2 to create 2D and 3D nonspherical polystyrene (PS) particle arrays of various shapes by using PS spheres stacking layer by layer, with the top layer acting as mask. One disadvantage of this process is that the area of the arrays with a certain configuration is small because there is no controllable method to fabricate large-area of certain layers of PS spheres until now. Tan et al.  and Yan et al.  prepared nonclose-packed polystyrene spheres by using a gas mixture of CF4 and low O2 content and pure argon plasma etching process, respectively. Only elliptical particles were obtained. Wu et al.  fabricated nano-net structure with necks formed between neighboring PS particles by oxygen plasma etching of a monolayer of PS spheres. However, the necks disappeared when the etching time was longer than 3 min, which leading to the uncontrollability of further manipulating the dimension of this novel nano-net structure.
In this work, we demonstrate a simple and inexpensive method to fabricate controllable nonclose-packed nonspherical PS particle arrays with long-range order. The method is based on a combination of colloidal self-assembly, preheating, and oxygen reactive ion etching techniques. The long-range ordered network pattern of PS particle arrays with tunable neck width and length were obtained. The hexagonal- and the rectangular-shaped PS particles were fabricated. Moreover, the round nanoholes were also achieved after oxygen RIE of double layer of PS spheres with preheating. These structures and patterns differ noticeably from the known elliptical-shaped PS particles and triangular nanoholes produced without preheating. Such unique colloidals and their ordered arrays resulted from the strategy demonstrated in this work may have important applications in fields of chemical sensors, photonic crystals, catalysts, biosensors, and can serve as good deposition or etching masks for growth of other 2-dimensional nanostructures, which have shape- and size-dependent properties. The effect of preheating on the fabrication of long-range ordered nonclose-packed nonspherical colloidal nanopatterns was also discussed in this work.
Monodispersed PS spheres (1,000 and 465 nm in diameter) suspensions (2.6 wt% in water, surfactant-free) were purchased from Polysciences, Inc and diluted by mixing with an equal amount of ethanol. The Si substrates were cleaned in an ultrasonic bath with acetone, ethanol, and deionized water at room temperature, and then rinsed using deionized water. A monolayer of highly ordered PS spheres were first self-assembled on water surface using a technique reported by Rybczynski et al.  as below. About 5 μL of prepared solutions was dropped onto the surface of a 3 × 3 cm large clean silicon wafer, which was kept in 10% dodecylsodiumsulfate solution for 12 h previously. The wafer was then slowly immersed in the Ø 10 cm glass vessel filled with deionized water and PS spheres started to form a monolayer on the water surface. Such monolayer was then lifted off from the water surface using another cleaned Si substrate, and dried in air at room temperature. Double-layered PS spheres were produced by immersing dry, once-covered substrates into water and lifted off a second layer. Then, the as-prepared monolayer of PS spheres with diameters of 465 and 1,000 nm were put into an airtight oven and preheated for 1 and 2 min, respectively. The airtight oven was heated up to 110 °C before putting samples into it, which is slightly higher than the glass transition temperature of PS (i.e., Tg = 100 °C, provided by the PS microsphere manufacturer). Finally, the RIE process was performed by using March PX-250 plasma etching system with power of 70 W and base pressure of 70 mTorr. Pure oxygen gas with flow rate of 100 sccm was used as plasma source to morph the preheated close-packed PS spheres monolayer into arrays of various nonclose-packed nonspherical PS particle patterns with varying RIE durations. The morphologies of the samples were characterized by field emission scanning electron microscopy (FE-SEM, JEOL JSM-6700F).
Results and Discussion
In summary, we have fabricated controllable PS particle structures with a long-range order by combination of preheating and oxygen RIE techniques. The neck length and neck width of the network pattern fabricated by oxygen RIE of preheated monolayer of PS spheres can be easily tuned from about 30 to 80 nm and 150 to 80 nm, respectively, by increasing the oxygen RIE time. Moreover, the hexagonal-shaped and rectangular-shaped PS particles and round nanoholes were obtained after oxygen RIE of monolayer and double layer of PS spheres with preheating, which differs noticeably from the elliptical-shaped PS particles and triangular nanoholes produced without preheating. The network pattern with controllable neck width and length and the hexagonal-shaped as well as rectangular-shaped PS particle arrays obtained with preheating are new colloidal lithographic nanopatterns, which raised hopes for NSL. Preheating plays a crucial role in fabricating these new long-range ordered PS particle arrays. These new colloidal nanopatterns have important applications in fields of catalysts, biosensors, and biomedical devices, especially in next-generation integrated nanophotonic devices, bimolecular labeling and identification .